### Politecnico di Torino ^{ }

Department of Mechanical and Aerospace Engineering

### Master’s Thesis In

### Mechanical Engineering

A.Y. 2021/2022 April 2022

**Finite Element Analysis Of Dental ** **Restorative Adhesives **

Supervisors: Candidate:

Prof. Giorgio Chiandussi Prof. Alessandro Scattina

Simon Arsene Nsegbe Mgbatou

To my mum and my late dad, forerunners of science in the family

In this thesis, 3-Dimensional Finite Element models were developed in LS-PrePost and then run in LS-DYNA in order to simulate three common mechanical tests very useful in the dentistry field. These tests are microtensile bond test, shear bond test and push-out test. For each of these tests, several 3-dimensional finite element models were developed with the aim to compare the experimental results to the results obtained from the nume- rical models. A particular attention was dedicated to the modelling of the cohesive zone in the different models. From LS-PrePost, the different geometries of the models were completely built then, the tiebreak contact was used as a first approach to model the cohesive zone in our models. The second approach consisted in using cohesive elements to model the cohesive zone in our models. The results obtained from the finite element analysis (FEA) of each model were analysed through the force-displacement curves mainly, and compared to the experimental results of these tests for the validation.

1 Introduction 9

1.1 Objectives and Purposes . . . 10

1.2 Method and Tools . . . 10

2 Microtensile Bond Strength Test 12 2.1 Literature Review and Experimental Test Description . . . 12

2.2 Finite Element Model with the Tiebreak Contact . . . 17

2.2.1 Geometry and Mesh . . . 17

2.2.2 Materials . . . 18

2.2.3 Boundary conditions . . . 18

2.2.4 Tiebreak Contact . . . 20

2.2.5 Results . . . 22

2.3 Finite Element Model With Cohesive Elements . . . 26

2.3.1 Geometry and Mesh . . . 26

2.3.2 Materials . . . 27

2.3.3 Boundary conditions . . . 29

2.3.4 Cohesive Elements and Elements Connectivity . . . 29

2.3.5 Results . . . 30

2.4 Comparison between the Tiebreak Contact and the Cohesive Elements . . 34

3 Shear Bond Strength Test 36 3.1 Literature Review and Experimental Test Description . . . 36

3.2 Finite Element Model With Tiebreak Contact . . . 38

3.2.1 Geometry And Mesh . . . 39

3.2.2 Materials . . . 40

3.2.3 Boundary Conditions . . . 41

3.2.4 Contact Between Parts . . . 42

3.2.5 Results . . . 44

3.3 Finite Element Model with Cohesive Elements . . . 46

3.3.1 Geometry and Mesh . . . 46

3.3.2 Materials . . . 47

3.3.3 Boundary Conditions . . . 48

3.3.4 Contact Between Parts . . . 49

3.3.5 Results . . . 51

3.4 Comparison Between the Different Approaches . . . 53

4 Push-Out Bond Strength Test 55 4.1 Literature Review and Experimental Test Description . . . 55

4.1.1 Literature Review . . . 55

4.1.2 Experimental Test Description . . . 56

4.2 Finite Element Model with the Tiebreak Contact . . . 60

4.2.1 Geometry and Mesh . . . 60

4.2.2 Materials . . . 62

4.2.3 Boundary Conditions . . . 63

4.2.4 Contact Between Parts . . . 64

4.2.5 Results . . . 66

4.3 Finite Element Model With Cohesive Elements . . . 69

4.3.1 Geometry and Mesh . . . 69

4.3.2 Materials . . . 71

4.3.3 Boundary Conditions . . . 72

4.3.4 Contact Between Parts . . . 73

4.3.5 Results . . . 74

4.4 Comparison Between The Different Approaches . . . 77

5 Conclusion 79

2.1 specimens preparation . . . 13

2.2 specimen mounted on the testing machine . . . 14

2.3 adhesive failure of the specimen . . . 16

2.4 mesh of the model . . . 17

2.5 model with boundary conditions . . . 19

2.6 Velocity load curve . . . 19

2.7 contact segments on dentin and ceramic . . . 21

2.8 Tiebreak contact zone: 121 of 121 nodes tied . . . 22

2.9 stress distribution on the structure in [Pa] . . . 23

2.10 Paths on the top surface for stress trend plots . . . 23

2.11 Von Mises stress distribution in [Pa] . . . 24

2.12 Paths on Cerasmart part for stress trend . . . 24

2.13 Experimental and Numerical Force-Displacement curve . . . 25

2.14 Geometry of the model with cohesive elements . . . 26

2.15 cohesive elements: node to node correspondence with surrounding parts . 27 2.16 no correspondence node to node . . . 28

2.17 Model with boundary conditions . . . 29

2.18 Von Mises stress distribution on the cohesive node to node model [Pa] . . . 31

2.19 Von Mises stress distribution on the cohesive tied contact model [Pa] . . . 31

2.20 Von Mises stress distribution in [Pa] on parts: cohesive elements with node to node correspondence model . . . 32

2.21 Von Mises stress distribution in [Pa] on parts: cohesive elements with tied contact model . . . 32

2.22 Force-Displacement curves node to node model . . . 33

2.23 Force-Displacement curves tied contact model . . . 34

2.24 Force-Displacement curves . . . 35

3.1 Dimensions of a generic specimen for the micro shear bond test . . . 38

3.2 Specimen mounted on the testing machine for the micro shear bond test . 38 3.3 Geometry of the model . . . 39

3.4 Shear bond test model: The mesh . . . 40

3.5 Boundary Conditions enforced on the model . . . 41

3.6 velocity enforced to the indentor . . . 42

3.7 segments sets for the tiebreak contact . . . 43

3.8 Von Mises stress distribution on the model [GPa] . . . 44

3.9 Von Mises stress distribution on each part[GPa] . . . 45

3.10 Force-Displacement curves . . . 46

3.11 Geometry of the model and mesh generated from the geometry . . . 47

3.12 Boundary conditions: Constrained nodes in white . . . 49

3.13 Contact between the indentor and the enamel . . . 49

3.14 segments set defined on the dentin and the adhesive for the tied contact . . 50

3.15 segments sets defined on the enamel and the adhesive for the tied contact . 50 3.16 Von Mises stress distribution on Enamel [GPa] . . . 51

3.17 Von Mises stress distribution on Dentin [GPa] . . . 51

3.18 Force-Displacement curves . . . 52

3.19 Force-Displacement curves . . . 53

4.1 Schematic drawing of the specimen preparation procedure for the micro- push-out bond strength test on 1 mm thick slices. (A)The crowns were removed 2 mm above the cemento-enamel junction (CEJ). (B) After the cleaning-shaping procedure, an adhesive root canal filling was performed. (C) Preparation of the post-space with pre-calibrated burs.(D) Cementa- tion of the fiber post into the root canal. . . 57

4.2 Schematic drawing of the specimen preparation procedure: slices obtained from each root canal. . . 58

4.3 Schematic drawing of the specimen mounted on the testing machine . . . . 58

4.4 Force-Displacement curve registered for the sample submitted to micro- push-out test. . . 59

4.5 Geometry of the model exploded with dimensions . . . 60

4.6 Isometric view of the model meshed: the part in red represents the mesh generated from the dentin, the part in green represent the mesh generated from the cement layer, the part in blue represents the mesh generated from the glass post and the part in yellow the mesh generated from the steel rod. 61 4.7 Down view of the model: constrained nodes highlighted in red . . . 63

4.8 velocity curve prescribed to the rod . . . 64

4.9 contact between the rod and the glass post . . . 64

4.10 Tiebreak contact defined on the two subgroups of parts . . . 65

4.11 Von Mises stress distribution on the model in [GPa] . . . 66

4.12 Von Mises stress distribution on the cement and the glass post in [GPa] . . 67

4.13 Von Mises stress distribution on the dentin in [GPa] . . . 68

4.14 Force-Displacement curves . . . 69

4.15 Geometry of the model . . . 70

4.16 Mesh generated from the parts . . . 71

4.17 Partial top view of the model . . . 73

4.18 Von Mises stress distribution on the whole model . . . 74

4.19 Von Mises stress distribution on the glass post and the cement in [GPa] . . 75

4.20 Von Mises stress distribution on the dentin in [GPa] . . . 75

4.21 Stress distribution on the cohesive layers in [GPa] . . . 76

4.22 Force-Displacement curve . . . 77

4.23 Force-Displacement curve . . . 78

2.1 Mechanical properties of the materials . . . 18

2.2 Equivalence between the parameters used by the solver algorithms for the two different approaches. The parameters belonging to the same row have the same physical meaning. . . 35

3.1 Dimensions of the parts and Mesh size of the elements . . . 39

3.2 Properties of the materials . . . 40

3.3 Equivalence between the parameters used by the solver algorithms for the two different approaches. The parameters belonging to the same row have the same physical meaning. . . 53

4.1 Mesh properties of the different parts . . . 62

4.2 Mechanical properties of materials . . . 62

4.3 Properties of the mesh for each part . . . 71

4.4 Equivalence between the parameters used by the solver algorithms for the two different approaches. The parameters belonging to the same row have the same physical meaning. . . 77

## Introduction

Nowadays, restorative dentistry appears to be one of the most developing areas of me- dical care, principally connected with the commonness of dental caries. By restorative dentistry we refer to any dental procedure that repairs or replaces a tooth. Restorative procedures include cavity fillings, root canals, and even dental implants. There can be two goals in restorative dentistry: the restoration of the function of the teeth and the restoration of the appearance of the teeth. In some cases it’s one or the other, and in some cases it’s both. Most often, the adhesive materials are used in the dentistry field and greatly contribute to the teeth restoration. MJ Tyas and MF Burrow state that adhesive restorative dentistry originated with the work of Michael Buonocore in 1955 in bonding resin to etched enamel. Buonocore was able to demonstrate that the treatment of enamel with phosphoric acid resulted in a porous surface, which could be infiltrated by resin, to produce a strong micromechanical bond. However, the clinical application of acid etching was not realized until 15years later when resin composites became available as a result of the work of Bowen’s group. In contrast to micromechanical bonding to tooth tissue, chemical bonding was developed by Smith and resulted in the introduction of polycarboxylate cement. Since then, adhesive materials and techniques have developed at a rapid rate. The first chemically adhesive material (zinc polycarboxylatecement) was marketed in the late 1960s, and glass-ionomer cements and dentine bonding agents have since become available [1]. The rapid development by companies of adhesive systems for the restorative dentistry gave birth to the necessity of characterize them in order to have a better knowledge of their properties. The adhesives used in the field of restorative dentistry have several properties but, the properties of interest for us are the mechanical properties. The mechanical properties of the restorative adhesives are evaluated through some tests such as microtensile bond strength test, shear bond strength test and push- out test. These tests are commonly used in the dentistry field for that purpose. The results obtained in the laboratories from these tests are considered to be good enough nevertheless, with the development of numerical methods for the resolution of physical problems described by partial differential equations, numerical models have been increa- singly built in recent years in order to have information that would have been difficult if

not impossible to obtain from the experimental tests.

### 1.1 Objectives and Purposes

The objectives in this thesis work is the analysis via the finite element method of different adhesive systems used in the restorative dentistry. This analysis needed to be performed through the microtensile bond strength test, the shear bond strength test and the push- out test. Therefore, it was necessary to build some numerical models for each of these tests. The building of the numerical model included the construction of the geometries, the generation of the mesh, the definition of all the material models which represent in the best way the real materials, the definition of all the contact experienced by the parts, the definition of the boundary conditions ...etc. Since, the attention was dedicated to the ad- hesive systems used in these models, the cohesive zones were modelled using two different approaches. The first approach used for the modelling of the adhesive in the model was the Tiebreak Contact. As the second approach, we used cohesive elements to model the adhesive systems in the different numerical models. These two adhesive models allowed us to have information such as the adhesive bond strength, the adhesive stiffness and the stress distribution on the parts surrounding the adhesive. The results obtained from these two adhesive models were compared then. The force-displacement curve obtained from each numerical model was compared to its correspondent experimental force-displacement curve for the validation.

### 1.2 Method and Tools

In this thesis, the analysis of restorative adhesives was performed via the finite element method. As it is widely known, the finite element method (FEM) is a numerical method widely used nowadays to solve physical problems in the fields like structural mechanics, heat transfer, fluid flow, mass transport, ...etc. Roughly speaking, to solve a problem, the FEM subdivides a large system into smaller and simpler parts from the point of view of the shape that are called finite elements. The finite element method is useful because it can give if well used some information which are accurate enough in particular when we are interested in information or phenomena regarding particular locations of a domain.

For this thesis, we opted for the software LS-DYNA to run the different models built in LS-PrePost which is the pre and post processing software of LS-DYNA.

LS-DYNA is an advanced general-purpose multiphysics simulation software package de- veloped by the former Livermore Software Technology Corporation (LSTC), which was acquired by Ansys in 2019. LS-DYNA’s potential applications are multiple and can be accommodated to many fields. LS-DYNA is not limited to any particular type of sim- ulation. In a given simulation, any of LS-DYNA’s features can be combined to model a wide variety of physical problems. Some features make LS-DYNA one of the main si- mulation software used to solve physical problems. Being a general purpose multiphysics

software, it can simulate a wide range of problems. Its material library is also a huge advantage for the analysts because it contains a very large material models which allows the analyst to easily find the material model which fit the best reality. Another advantage in using LS-DYNA is the possibility to choose in between several contact algorithms to model the contacts and interactions between parts in a model. The capability to predict accurately events which involve large deformations such as car’s behavior in a collision, sheet metal forming...etc makes it one of the softwares most used for these applications in the industry. The main solution method implemented in LS-DYNA is the explicit time integration. The implicit solver is also available but presents a lot of limitations because a lot of features such as contact algorithms, element formulations...etc are not available for the implicit solver. For this work, all the simulations were realized using the version LS-DYNA R9 Finite Element explicit solver.

## Microtensile Bond Strength Test

### 2.1 Literature Review and Experimental Test Des- cription

Many laboratories use tensile bond tests to compare adhesive systems or evaluate the
influence of experimental variables on restorative material-dentin bond strength. Gene-
rally, they limit the location of the bond to the center of the occlusal or labial surface
of midcoronal normal dentin. The bonded surface is demarcated using a 3 mm or 4
mm diameter hole punched in sticky tape, or some type of matrix is used that is 3
to 4 mm in diameter (7 to 12 mm^{2}). These simple tests served well when restorative
material-dentin bond strengths were relatively low (circa 10 to 15 MPa). However, as
bonding techniques and materials improved, the bond strengths became high enough to
cause cohesive failures in dentin or in the restorative material. That is, dentin broke
from dentin, leaving the restorative material dentin interface intact or the restorative
material broke leaving the dentin-resin bonded interface intact. The frequency of cohesive
failures of dentin for instance can be as high as 80% when bond strengths reach 25 MPa.

Such failures of the substrates preclude measurement of interfacial bond strengths and limit further improvements in bonding formulations, since the tests can no longer detect improved adhesion. Such cohesive failures in dentin or even in the restorative material do not mean that the restorative material-dentin are uniformly stronger than the intrinsic strength of dentin, but that the way in which the bond is stressed is so non-uniform that it is concentrated or focused at one highly localized region where it opens a crack either in dentin or in the restorative material, that then fails [2]. These stress concentrations often exceed 10 MPa, even though the calculated average bond strength is only 32 MPa.

To avoid cohesive failures of dentin during bond testing, it is necessary to improve stress distributions during testing. This can be accomplished by the microntensile bond testing method. It is a labor-intensive method than the conventional method but avoid inducing cohesive failures in dentin. This method tends to lower the variance associated with testing

to 10% to 25%, instead of the more common 30% to 50% variance seen in conventional testing. Since it may be difficult to obtain extracted teeth, especially intact premolars and

Figure 2.1: specimens preparation

third molars, the microtensile testing method allows multiple specimens to be prepared from each tooth (fig:2.1). Therefore, there is a compromise between the extra labor involved in using this method and the extra data that can be obtained per tooth.

Microtensile bond testing was originally designed to permit evaluation of bond strengths
between adhesive materials and small regions of dental tissue(eg, occlusal vs middle vs
cervical third of enamel, normal vs adjacent caries-affected dentin, occlusal vs gingival
walls of Class vs wedge-shaped lesions). One advantage of the technique is that the bonded
interface of small specimens (about 1mm^{2}) has a better stress distribution during loading,
so that there are fewer cohesive failures in dentin than are found with more conventional
testing. This is thought to be due to a reduction in flaw density. Using this method often
results in higher apparent bond strengths at failure than are found using large specimens.

Since the introduction of the technique, a number of laboratories have made numerous modification to it.

The original microtensile testing was done on mineralized dentin to measure its ultimate tensile strength (UTS) and modulus of elasticity.To measure the ultimate tensile stress, the specimens were trimmed to an hourglass profile to produce uniform stressing of the smallest cross-sectional area. To measure the modulus of elasticity in tension, the need

of a known gauge-length required that the specimens be trimmed to the outline of an

”I” beam. That approach has also been used to measure the ultimate tensile stress and elastic modulus of the demineralized dentin matrix by protecting the mineralized ends of the specimens with nail varnish, while the central region was demineralized in EDTA.

Nowadays, several adhesive systems are used in the dentistry field. With the microtensile bond strength test, scientists can measure the strength of the bond due to the adhesive system in the restorative dentistry. The essence of the microtensile test is therefore the division of resin-bonded teeth into slabs 1.0 mm thick that are then trimmed in such a manner that tensile force will be concentrated on the bonded interface during testing.

Among the many advantages of the technique as we said are that each tooth produces

Figure 2.2: specimen mounted on the testing machine

multiple specimens. Further, there is no need for a matrix to limit the bonded surface area, since the area is determined by the dimensions of the trimmed specimens.

It is also important to say that so far, no standard test has been approved for measuring the bond strength of dentin and composite using dental adhesive system. Different test methods and parameters used have resulted in discrepancy of the data reported by dif- ferent researchers on the same adhesive system. The factors affecting the bond strength have been addressed by few researchers before. Pashley et al have listed these factors in a review paper under the broad categories of substrate variables, etching variables, priming variables, bonding variables, storage variables and testing variables. Most of this review has focused on the issues relating to the differences induced by the material properties or the process used in sample preparation. The substrate and adhesive variables induce inherent differences in the material properties. Data reported on the dentin and bovine strength can be up to 50% different depending on the source and part of the dentin or bovine used. The same sort of data spread is reported for demineralized dentin, with some data on the strength being almost one-third of the other test data. The process

used in the preparation of the sample as well such as etching and priming have effect on the interface properties and therefore on the bond strength.

Van noort et al. [3-4] have analyzed the effect of the test method in the bond strength results. They have made a comparison between the microtensile test and shear test in measuring bond strength. Applying FEA they have concluded that the shear test results in unfavorable stresses in the specimen. Consequently, they have recommended the tensile test as a preferred test method for measuring bond strength. While the advantages of the microtensile test were proved, many researchers applied the method to measure the bond strength of dental adhesive [5-6]. Nakabayahsi et al. [7] apply the method to detect defects in the specimen. They study the effect of defects in the failure characteristics of the miniaturized samples. Capel Cordoso et al. [8] use the microtensile bond strength to compare the bond strength of three adhesive systems with the cohesive strength of dentin and composite. In all three systems they find the adhesive bond strength to be much lower than the strength of composite or dentin. Yoshiyama et al. [5] apply the microtensile test to measure the bond strength to different regions of dentin. They have reported higher bond strength on the coronal and apical dentin compared to the bond strength to the cervical root dentin. The effect of specimen size and geometry in the re- sults of the bond strength is studied partly by other researchers[4]. Phrukkanon et al. [9]

have investigated specimens with round and rectangular cross sections. For four different adhesive systems they have reported higher bond strength for the circular cross section compared to the rectangular cross section. The second parameter they have considered is the cross sectional area of the samples. For three different cross sections, lower bond strength is estimated for larger cross sections. The results have been explained using FEA to estimate the stress distribution. They have attributed this result to higher stress val- ues for the samples with larger cross section. Other researchers have used Griffith theory to explain the same results. They have reasoned that smaller samples will have smaller flaw size and therefore higher strength. In Phrukkanon’s research they have increased the surface area without changing any other part of the sample. If they scale up all parts of the sample with the surface area the FE results would not indicate any changes for different surface areas. Whereas experimental tests still indicate smaller strength for the samples with larger cross sectional area. This shows a second parameter having role in reducing the bond strength for the larger size specimens which is recommended by Griffith’s theory. Although the researchers have highlighted the parameters affecting the result of the bond strength in the previous studies, there is little indication of quantifying each effect and systematic study. At the same time most of the previous researches on the factors affecting the result of the bond strength have identified only one or two pa- rameters, ignoring the other parameters. Elaheh Ghassemieh has considered broad range of factors affecting the bond strength and modes of failure. Using finite element analy- sis he has investigated the effect of each parameter on the general stress distribution in different regions of adhesive, at the interface of the adhesive and composite and at the interface of adhesive and dentin. He has quantified the effect of each variable on the bond strength and modes of failure for the most commonly used geometries of stick, dumbbell and hourglass. He stated that the advantage of using finite element analysis to study

Figure 2.3: adhesive failure of the specimen

and evaluate the sources of uncertainties in microtensile bond strength of dental adhesive system for different specimen geometries is that, it makes separation of the parameters and its effect possible. The experimental tests do not allow to isolate the different factors that might influence the bond strength and therefore, interaction of the variables which influence the microntensile bond strength test is normally unavoidable. The final FEA predictions of bond strength, its variations and modes of failure are derived from bring- ing together the results of analysis for all the identified individual parameters. Elaheh Ghassemieh [4] performed microtensile bond strength experiments in order to validate the FEA estimation of the mode of failure, bond strength and its standard deviation for the mentioned geometries. His results showed that the experimental measurements of these parameters and the ranking of different geometries in bond strength approve the collective predictions of FEA and confirmed the reliability of the finite element analysis in its estimation of other individual effects as well.

We can say that the microntensile bond strength test consist in mounting a specimen with 1mm X 1mm cross section on a testing machine as shown in figure 2.2.

Then, an axial load is applied to the specimen in other produce a stress state in the specimen which will caused the failure of the specimen. As we already stated, it is necessary to have an adhesive failure (fig2.3) of the specimen in order to evaluate the

tensile bond strength dividing the peak of the axial force registered by the cross section area of the specimen.

### 2.2 Finite Element Model with the Tiebreak Contact

Two approaches were used to model and simulate the microtensile bond strength test in order to characterize the adhesive system used in restorative dentistry. The main difference between the two models corresponding to the two approaches that we used lies in the modelling of the cohesive zone of our models. Here is the description of the first approach based on the modelling of the cohesive zone of our model with the Tiebreak Contact in LS-DYNA.

### 2.2.1 Geometry and Mesh

The pre-processing step was performed in LS-PrePost (LSPP) which is an advanced pre- and post-processor and model editor from LSTC, preparing input data for LS-DYNA.

Concerning the geometry, the useful information was the dimensions of the parts consti- tuting our model. The experimental test allowed us to have a clear idea on the geometry of our model. Therefore, Two solid parts with dimensions 1mm × 1mm × 5mm were modelled in LS-PREPOST, then we generated a three dimensional solid mesh from the two parts since they are solid (fig2.4). In order to have a realistic mesh of our model, the meshes generated from the two parts of our model were different from the point of view of the mesh size. This choice was made in order to have a more realistic contact simulation between the two parts as we will see later. Therefore we chose a mesh with a maximum

Figure 2.4: mesh of the model

element size of 0.14mm for the part in red which represents the dentine while, we chose

a mesh with a maximum element size of 0.1mm for the part in blue which represents the enamel. Once we generated the mesh of our model, we assigned to the elements of our model an element formulation among those proposed by LS-PrePost. Being the parts of our model with regular geometries, we opted for hexahedron elements with element formulation ELFORM=3. This choice of the element formulation is justified by the fact that ELFORM 3 are fully integrated solid elements therefore, such elements prevents us from having hourglass modes.

### 2.2.2 Materials

The model of the experimental test was constituted by dentine, cerasmart and a cement known as PANAVIA V5. In this three dimensional finite elements analysis, all the parts of our model were considered homogeneous, linear, and isotropic. For this reason, in the LS-DYNA material library, all the materials were modelled with the MAT 001 which corresponds to MAT ELASTIC and is an isotropic elastic material which is available for beam, shell, and solid elements in LS-DYNA. The mechanical properties useful for the finite element analysis are given in the table 2.1.

Materials Young’s Modulus(GPa) Poisson’s Ratio

Dentin 18 0.31

Cement 1 0.30

Cerasmart 69 0.28

Table 2.1: Mechanical properties of the materials

Perfect adhesion between the ceramic (cerasmart) and the cement and between the cement and dentin was assumed. The choice of the material behaviour and properties is motivated by the choice made in all the previous studies that were found in the literature.

### 2.2.3 Boundary conditions

The definition of the boundary conditions on our model was performed in order to simulate in the best possible way the boundary conditions enforced during the experimental test.

It is worth to say that previous studies have been performed in order to understand how the boundary conditions enforced on the numerical model can affect the results of the simulation. These previous studies demonstrated that boundary conditions affect not only qualitatively the results of the microtensile bond strength test, but also quantitatively.

In our case, the experimental text allowed us to constrain all the degrees of freedom of the nodes belonging to the elements going from the base to 1mm of the dentin just like we can see the nodes highlighted in white in the figure 2.5. Since we opted for an explicit analysis, it was necessary to enforce a displacement law on the nodes belonging to the elements going from 9mm to 10mm (being the base of the dentine the origin of our frame

Figure 2.5: model with boundary conditions

of reference). The velocity enforced on those nodes in order to generate the load is shown on the figure 2.6. We had the choice to enforce either a constant velocity on the moving

Figure 2.6: Velocity load curve

nodes or a linear velocity, but we opted for a smoothly changed velocity curve. Such a load curve was chosen in order to avoid significant accelerations during the loading of the structure. Significant accelerations during the loading phase would have introduced dynamic effect on the model that we needed to avoid. It is also important to highlight the fact that the experimental test is performed with a loading machine moving at around 5mm/min. Such a velocity is too low for an explicit analysis because it requests a very long simulation time which is directly linked to the CPU time. Therefore, we decided to accelerate the numerical test in order to reduce the CPU time namely reduce the computational cost.

### 2.2.4 Tiebreak Contact

In order to simulate the adhesive interface between the dentin part and the ceramic part of our model, we opted in a first attempt for a Tiebreak Contact type in LS-PrePost. going to the keyword contact in LS-PrePost, we have the choice between several possibilities of contact.

The CONTACT AUTOMATIC SURFACE TO SURFACE TIEBREAK was chosen to model the cohesive zone in our model. In general, to completely model the cohesive zone, several parameters have to be set in the right way. Here follow the parameters that were used to completely define the cohesive zone.

• Option 6: in the contact card we had to chose an option for the contact that we chose. The choice of this option was based on the description given by LS- DYNA Manual Volume I R12. From the manual volume, we can notice that option 6 is suitable for the use with solids and thick shells elements only. Tiebreak is active for nodes which are initially in contact. Failure stress must be defined for tiebreak to occur. After the failure stress, tiebreak criterion is met. damage is a linear function of the distance between points initially in contact. When the distance is equal to PARAM, damage is fully developed, and interface failure occurs. After failure, this option behaves as a surface-to-surface contact. Since our model is made of solid elements, this option is suitable for our model.

• NFLS: for the option 6 that we have just seen, NFLS represents the normal failure stress of the adhesive. The value of the normal failure stress was unknown but a value of 46 MPa was chosen in order to guarantee the microtensile bond strength given by the experimental test.

• SFLS: it represents the shear failure stress in the contact card. For the microtensile bond strength test, SFLS is not very important because the shear stress in this model is very low therefore, it does not really influence the failure of the contact.

• PARAM: for option 6, PARAM is the critical distance (CCRIT), at which the inter- face failure is complete. Since we did not have the experimental force- displacement curve, such a parameter was not important for our analysis.

• CT2CN: it represents the ratio of the tangential stiffness of the adhesive to the normal stiffness of the adhesive. This was set to be equal to 1. This parameter was not very important for the analysis since the microtensile bond strength test normally a pure mode.

• CN: is the normal stiffness (stress/length) for OPTION = 6. If CN is not given explicitly, the penalty base approach that we will discuss later on is used to define the normal stiffness dividing the penalty stiffness divided by segment area (default).

The manual recommends the use of this option with care, since contact stability can get affected. A value of 18500 GPa/m was assigned on the basis of the Young’s modulus of the adhesive systems used during the experimental test.

Now that we have all the variables influencing the cohesive zone in our model, let us see how damage and failure occur in the tiebreak contact option that we chose. The tiebreak failure criterion has normal and shear components and is given by the following relation:

σ_{n}
N F LS

2

+ σ_{s}
SF LS

2

≥ 1 (2.1)

Whereby σ_{n} is the tensile normal stress and is taken as zero if the normal stress is
compressive while σ_{s} is the shear stress. Damage initiates when the stress meets the
failure criterion. We can easily note from the relation 2.1 that in case the shear stress σ_{s}
is very low, the second term at the right member of the relation will tend to zero therefore,
the damage will be ruled almost only by the normal stress σ_{s}.

In LS-DYNA, in order to define the contact between parts of a model, we need to decide whether the contact will be of type node to node, segment to segment or part to part.

(a) Dentin contact surface (b) Ceramic contact surface Figure 2.7: contact segments on dentin and ceramic

This has to be defined when we have decide the slave and master side of a contact in general. The right choice depends on the model and on the type of contact the analyst is dealing with. LS-DYNA manual recommends that the slave and master sides of tiebreak contact be defined using segment sets rather than part or part set. By doing this, we can be more selective when choosing which segments are to be tied and ensure that contact stresses calculated from nodal contact forces are not diluted by segments that are not actually on the actual contact surface. We also have more direct control over the contact segment normal vectors when segment sets are used. Segment normal vectors should point toward the opposing contact surface so that tension is properly distinguished from compression.

Checking the contact zone, we can realize that LS-PrePost give the message 121 of the 121 nodes are tied (fig2.8). This means that all the nodes of the part which has a higher mesh density are tied to the surface of the dentin part which has a lower mesh density.

Figure 2.8: Tiebreak contact zone: 121 of 121 nodes tied

### 2.2.5 Results

After all the pre processing steps performed on LS-PrePost that we just described, the simulation was run through the cluster of the HPC@POLITO, a powerful tool furnished by the Politecnico di Torino and managed by the Department of Automation and Com- puter Science (DAUIN) of the Politecnico. That corresponds in calculation resources and technical support for academic and didactic research activities using centre systems. The cluster used in this thesis work was Legion cluster. The simulation was completed in 35 minutes and 48 seconds with 64 cores on 2 nodes. Here follow the main results obtained from the simulation after the post processing on LS-PrePost.

2.2.5.1 Stress Distribution

Von Mises stress distribution on the entire model shows that the stress is almost null at the ends of our structure. Then from both the sides of our structure, the closer we are from the cohesive zone of the model, the higher is the stress (fig2.9).

We also plotted Von Mises stress distribution in z direction along all the structure. The first path regards the stress distribution in z direction at almost the center of the model on the top surface as shown in figure 2.10a While the second path was chosen in order to

Figure 2.9: stress distribution on the structure in [Pa]

represent the stress distribution in z direction but this time at an edge of the structure (fig 2.10b).

(a) Central path (b) Edge path

Figure 2.10: Paths on the top surface for stress trend plots

Since the stress distribution is almost symmetric in each part of the model in all the directions, it was not necessary to plot and represents the stress distribution along other paths since the one we represented are already describing the whole structure quite well.

The stress trend along the paths we just mentioned shows us that the maximum stress is located at the edge of the structure around the contact interface (at 5mm) as shows figure. In fact we can realize that the green curve which represents the trend at the edge has its maximum at the distance 5mm and the value is 64.7 MPa. We can also realised

that along the central path, the maximum stress is around 50 MPa. This result allows us to deduce that the failure begins at the edges of the contact interface. In the same way, we tried to figure out the difference in stress distribution on the parts constituting our model. We realized that the restorative material (Cerasmart) has higher stress values with respect to the dentin.

(a) Dentin (b) Cerasmart

Figure 2.11: Von Mises stress distribution in [Pa]

Since the maximum stress is located on the Ceramic part of the model, we were interested in understanding how is distributed the stress at the tiebreak contact interface on the restorative material. Just like in the case of stress trend in z direction on the top surface, Two paths were chosen in y direction.The first path was chosen in order to represent the stress trend at the center of the contact area while the second one was chosen in order to represent the stress trend at the edge of the contact area.

(a) central path (b) edge path

Figure 2.12: Paths on Cerasmart part for stress trend

Due to the simmetry of our model, we know that this two paths that we chose in y direction at the contact surface of our model are enough to have a clear idea on how is distributed the stress at the tiebreak contact interface which simulates the adhesive.

We have a same trend for the dentin part with the only difference that the dentin part is less stressed with respect to the cerasmart part. It worth to precise that the stress trends along all the paths that we plotted is just an indication of the stress distribution on the path. In order to obtain more realistic curves, it its necessary to have a finer mesh in such a way that we can have enough point on the curves.

2.2.5.2 Force-Displacement Curves

From the post processing, the force-displacement curves were also plotted in order to validate the numerical model, by comparing the experimental curve to the numerical curve that we obtained. From the experimental test. From the experimental test, we were able to obtain the adhesive tensile bond strength which is 32,58 MPa for PANAVIA V5. To the value of the tensile bond strength, we were also able to find the adhesive Young modulus which is given in table 2.1. The experimental value of the adhesive Young modulus combined to the value of the tensile bond stress allowed us to have the experimental force-displacement curve. The same value of the adhesive stiffness was introduced in the solver algorithm as the stiffness of the tiebreak contact.

Figure 2.13: Experimental and Numerical Force-Displacement curve

From the figure 2.13 we can realize that the peak of the force obtained from the numerical
results is 32,5 N. Considering the contact area of our model which is 1mm^{2}, we computed
the microtensile bond strength test from the equation and we obtained the value 32,5 MPa.

The numerical value of the tensile bond strength is quite close to the value obtained from

the experimental test which is 32,58 MPa. We can also say that the slopes of both the curves which depend on the stiffness of the model are fairly close. For what concerns the peak of the force, it is worth to say that the value of 32,5 N obtained from the numerical results was possible after running the model with different adhesive normal failure stress (NFLS). Therefore, several models were run inserting each time a different value of the adhesive normal failure stress up to reach the right value of the traction peak. Concerning the slope of the numerical force-displacement curve, we realized that by inserting material proprieties and by setting as the tiebreak contact stiffness the experimental stiffness of the adhesive, the results is quite close to the experimental one without the need of tuning the curve.

### 2.3 Finite Element Model With Cohesive Elements

The second approach that was used to model the microtensile bond strength test is the use of the cohesive elements within the model. The main difference between this approach with respect to the first one is the use of cohesive elements to simulate the adhesive within the model instead of a contact between the two parts constituting our model.

### 2.3.1 Geometry and Mesh

The geometry for this model with cohesive elements is almost the same with the previous one because the main parts of the model (dentin and cerasmart) have the same dimensions.

However, a new part was inserted in the model in between the two main parts in order to simulate the adhesive. The dimensions of this third part of our model representing

Figure 2.14: Geometry of the model with cohesive elements

the adhesive are 1mm × 1mm × 0, 05mm. These dimensions were chosen on the basis of the experimental test since the adhesive thickness during the experiment was 50µm.

On this geometry, two different mesh were generated in order to use two different contact algorithms proposed by LS-DYNA when using the cohesive elements. The first mesh we generated from this geometry is comprised of three parts with same element size in the XY plane. This was done in order to have a node to node correspondence between the parts. The second mesh that we generated from the geometry has the three parts of the model with different elements size in the XY plane. This second mesh was generated on the geometry in order to use a tied contact between the three parts. From figure 2.15, we can see that each node of the dentin (part in red) is located exactly in correspondence to a node of the cohesive elements representing the adhesive layer. In the same way, all the faces of the cohesive elements have their nodes which are located exactly in correspondence of the nodes of the ceramic cross section in contact with the adhesive. In this way, after the mesh generation, all these nodes sharing almost the same location were merged and the whole model behaves as a unique part after such a practice. Unlike the node to node

Figure 2.15: cohesive elements: node to node correspondence with surrounding parts correspondence model, where it is possible to merge the nodes sharing the same position, it is necessary in case we want to have a dissimilar mesh (fig 2.16) to enforce a tied contact in between the parts of the model. If such a practice is not performed, there is no way to use cohesive elements in LS-DYNA in case of non symmetric mesh at the cross section areas.

### 2.3.2 Materials

The materials used in this approach are almost the same with the one used with the tiebreak contact approach. For the dentin and the ceramic parts, we modelled them as linear elastic isotropic materials as it is recommended in the literature. In LS-PrePost the material model behaving like a linear elastic isotropic material can be chosen under the

Figure 2.16: no correspondence node to node

keyword MAT as 001-ELASTIC. Concerning the adhesive layer represented by the cohe- sive elements in the model, we assigned a material model known as 184-COHESIVE ELAS- TIC in LS-PrePost. In order to completely define this material the user must give a value for the following properties of the material.

• RO: From the manual user, we know that RO is the mass density. from the litera-
ture, we were able to find the value of RO equal to 1200Kg/m^{3}.

• ROFLG: it is a flag which tells whether density is specified per unit of area or volume. if ROF LG = 0, it specifies the density is per unit of volume (default) while if ROF LG = 1 specifies that the density is per unit of area for controlling the mass of cohesive elements with an initial volume of zero. This parameter is important because in LS-PrePost, zero thickness cohesive elements can be modelled and usually such a part should have ROF LG = 1. In our case, the adhesive thickness is 50µm therefore we opted for ROF LG = 0.

• INTFAIL: it is the number of integration points required for the cohesive element to be deleted. If it is zero, the element won’t be deleted even if it satisfies the failure criterion. The value of INTFAIL may range from 1 to 4, with set INTFAIL=1 because of the recommendation from the manual.

• ET: From the manual, we can read that ET is the stiffness in the plane of the cohesive element. This stiffness is expressed in the unit of stress/length. We can conclude that such a value corresponds to E/L namely the ratio between the adhesive Young’s modulus and the thickness of the adhesive. For the microtensile test, ET value is not really important since the traction is mainly normal to the plane of the cohesive element.

• EN: It is the stiffness normal to the plane of the cohesive element (stress/length).

From the properties of the adhesive, we set this value equal to 18500GPa/m.

• FN FAIL:It is the traction in the normal direction for tensile failure. This value was set to be equal to 33 MPa.

• FT FAIL: FT FAIL is the traction in the tangential direction for shear failure is necessary in case of cohesive the presence of the shear mode failure. The algorithm does not require this value for the microtensile bond test.

### 2.3.3 Boundary conditions

The boundary conditions enforced on this model with cohesive elements were the same with the one enforced on the model with the tiebreak contact. Such a choice was made in order to have comparable results between the different approaches. The loading curve

Figure 2.17: Model with boundary conditions

was chosen in order to have a test not too slow in order to reduce the simulation time, but at the same time not too quick in order to reduce dynamic effects during the simulation.

We can refer to figure 2.6 for information related to the velocity loading curve for the microtensile bond strength test.

### 2.3.4 Cohesive Elements and Elements Connectivity

In the LS-DYNA manual user, we have information related to the use of cohesive ele- ments. Among the possible element formulations available in LS-DYNA, just few of them can be used for cohesive elements. We opted for the element formulation ELFORM 19

because such a formulation is recommended in case the adherends are discretized with solid elements.

A cohesive element formulation connects via nonlinear spring elements the relative dis- placements between the upper and lower surface to a force per unit area. The element is really two dimensional. Instead of strains, the deformation is in terms of the relative displacements between the upper and lower surfaces interpolated to the Gauss points.

Unlike strains, the incoming deformations have units of length. The output of the mate- rial model is the force per unit area (LS-DYNA manual: traction) at the Gauss points, acting to oppose the displacement.

The two element formulations in LS-DYNA, which can be used with cohesive material models are ELFORM 19 and ELFORM 20. ELFORM 20 transfers moments between the bonded parts, whereas ELFORM 19 does not. The order of the nodes in defining the element is important. For instance if the cohesive element bonds Element A of the first adherend to Element B of the second adherend, nodes 1-2-3-4 of the cohesive element should be shared by Element A or by Element B. In the first case, the normal of face 1-2-3-4 should point towards Element B and nodes 5-6-7-8 should be shared by Element B. In the second case, the normal of face 1-2-3-4 should point towards Element A and nodes 5-6-7-8 should be shared by Element A. Any other kind of connectivity between the cohesive elements and the elements belonging to the adherends will produce errors during the simulation process and lead to the failure of the simulation. It is worth to say that the cohesive element formulations can have zero thickness and even invert without becoming unstable. Therefore, even very thin layer of adhesives can be modelled with these element formulations. Cohesive element is represented in the manual as consisting of three nonlinear springs (one in the normal direction and two in the two shear directions).

### 2.3.5 Results

Just like for the case of the first approach we have just seen,From the post processing we were able to obtain the stress distribution history and the force-displacement curves.

2.3.5.1 Stress Distribution

From the history of the Von Mises stress distribution, we were interested in the stress distribution on the parts of the model at the instant just before the failure of the structure.

The model node to node shows a value of the maximum stress of 43.79 MPa. The model cohesive tied contact instead ha maximum value of the stress equal to 44.16 MPa.

Figure 2.18: Von Mises stress distribution on the cohesive node to node model [Pa]

Figure 2.19: Von Mises stress distribution on the cohesive tied contact model [Pa]

Figure 2.18 and figure 2.19 show us that the stress distribution on both the models using cohesive elements is similar at least for what concern the stress distribution on the outer surfaces of the models.

In order to understand better how the stress is distributed on each part at the instant before the failure, and whether there is a difference or not in the stress distribution at the adhesive interfaces, it was necessary to display each part separately. The stress distribution on the parts of the node to node model (2.20) shows us that the maximum stress is located on the cerasmart part. We can also realize that even if the stress is more concentrated on the surfaces edges of the part in contact with the adhesive, there is not a huge difference in between the stress at the edges and the stress at the center of the surfaces. Just like the node to node model, The stress distribution on the cohesive with

(a) dentin (b) Cerasmart

Figure 2.20: Von Mises stress distribution in [Pa] on parts: cohesive elements with node to node correspondence model

tied contact between the parts (fig 2.21) shows us that the maximum stress is localized on the cerasmart. On the surfaces having a physical contact with the adhesive, we note that the stress is concentrated at the edges of those surfaces but the difference between the stress at the edges and the stress at the center is presumably less than 5 MPa.

(a) dentin (b) Cerasmart

Figure 2.21: Von Mises stress distribution in [Pa] on parts: cohesive elements with tied contact model

2.3.5.2 Force-Displacement Curves

From the post processing, the force-displacement curves were plotted in order to validate
the numerical model, by comparing the experimental curve to the numerical curve that we
obtained from the experimental test. As we already know, from the experimental test, we
were able to obtain the adhesive tensile bond strength which is 32,58 MPa for PANAVIA
V5. To the value of the tensile bond strength, we were also able to find the adhesive
Young modulus. The experimental value of the adhesive Young modulus combined to the
value of the tensile bond stress allowed us to have the experimental force-displacement
curve. The same value of the adhesive stiffness was introduced in the solver algorithm as
the stiffness of the cohesive material. From the figure 2.22 we can realise that the peak
of the force obtained from the numerical results is 32.2 N. Considering the contact area
of our model which is 1mm^{2}, we computed the microtensile bond strength test from the
equation 2.2 and we obtained the value 32.2 MPa.

### σ

_{T BS}

### = F

### A (2.2)

The numerical value of the tensile bond strength is quite close to the value obtained from the experimental test which is 32,58 MPa. We can also say that the slopes of both

Figure 2.22: Force-Displacement curves node to node model

the curves which depend on the stiffness of the model are almost the same. For what concern the peak of the force, it is worth to say that the value of 32.2 N obtained from

the numerical results was possible after running the model with different adhesive normal failure stress. Therefore, several models were run inserting each time a different value of the adhesive normal failure stress up to reach the right value of the traction peak.

Doing the same operation with the cohesive model used with tied contact and setting the same variables for the cohesive material in the algorithm, we obtained a similar force- displacement curve that is shown in figure 2.23. The curve shows a peak of the force equal to 31.9 N which corresponds to a tensile bond strength of 31.9 MPa.

Figure 2.23: Force-Displacement curves tied contact model

### 2.4 Comparison between the Tiebreak Contact and the Cohesive Elements

We recall that two approaches were used to model the adhesive layer. For each of these adhesive models, it was necessary to define some properties characterizing the model such as the stiffness of the adhesive, its failure stress... etc. Even if these parameters have different names in the manual user for each method, each parameter used to define the tiebreak contact has an equivalent parameter used to model the adhesive with the cohesive elements. The table 2.2 shows us that the main information necessary to model an adhesive with these two approaches are the adhesive failure stress in the normal and tangential direction as well as the adhesive stiffness. These values are enough when using these two approaches because they model adhesives with linear elastic models. We can

Microtensile bond strength test Tibreak contact Cohesive elements NFSL=46 MPa FN FAIL=33 MPa SFLS=10 MPa FT FAIL=10 MPa CN=18500 GPa/m EN=18500 GPa/m

Table 2.2: Equivalence between the parameters used by the solver algorithms for the two different approaches. The parameters belonging to the same row have the same physical meaning.

note from the figure that all the curves have almost the same slope.

The figure 2.24 shows us the force-displacement curves obtained from the numerical analy- sis for different approaches. We can deduce from this that both the methods are suitable to define the adhesive stiffness since the slope of each curve depends on the adhesive stiffness. Another observation is that the peak forces are almost the same. If we look

Figure 2.24: Force-Displacement curves

at the equivalence between the parameters (tab 2.2 used to simulate the adhesive layer, for the adhesive normal failure stress (NFSL) a value of 46 MPa was assigned whereas a value of 33 MPa was assigned with the cohesive elements approach to obtain the same peak force. From this observation we can say that the adhesive failure stress is probably between the two values.

## Shear Bond Strength Test

### 3.1 Literature Review and Experimental Test Des- cription

In-vitro mechanical tests of dental restorative materials provide dental practitioners with guidance as regards material selection criteria and identifying patterns of optimal clinical use of material. In vitro tests play a significant role in providing the necessary information regarding the effectiveness of new materials with less cost and in a short period of time, whereas clinical studies would provide information only after the use for long period. The quality of adhesive material bonding is frequently verified by various laboratory tests, using shear and tensile efforts under certain limitations [10-11]. In 1997, a study evaluated 50 studies that used laboratory tests to quantify the bond strength at the bond interface, and observed that 80% used the shear bond strength test in its several forms [12]. Today, use of the micro shear bond strength tests have increased considerably. However, several recent studies still use the shear bond strength test to evaluate adhesive material bonding.

In some situations, sectioning of the specimen for micro shear bond induces its loss due to failure before the test, and micro shear bond strength test cannot be used because of the difficulty of making specimens with some materials.In these cases, the shear bond strength test may be used to evaluate adhesive material bond strength. It is important to consider the changes in the test procedures commonly applied in different investigations that have the same aim: to determine the bond strength. For this reason, analyses of the same material inevitably produce different bond strength data [11,13-16].

Bond strength is obtained from the load at failure divided by the cross-sectional area of the bonded interface, and is referred as ‘nominal’ or ‘average’ bond strength. Shear bond strength tests have been widely used, mainly because of their relative simplicity when compared to tensile bond strength tests, in which it is difficult to align the specimen in the testing machine without creating deleterious stress distribution [17-19]. Advantages in shear tests include ease of specimen preparation and simple test protocol. However,

problems related to the validity of obtained measurements started to arise as cohesive failures in the substrate were frequently observed with new adhesives that yield improved bond strengths. Although some authors speculated that the bonding had surpassed the cohesive strength of the substrate with no further need for improvement, the actual con- clusion was that this test had turned out to be unsuitable to determine the true strength of a bonded interface [9,20]. According to Della Bona and van Noort [3], the real ex- planation for this fact was that stresses were mostly concentrated in the substrate, thus causing its premature failure prior to the interface itself. Another point that has drawn fundamental criticism regards to the non-uniform nature of stress distributions along tested interfaces [19]. According to a study performed by van Noort et al. [21] using finite element analysis to compare shear and tensile tests, the nominal bond strength may vary with specimen geometry, loading configuration and material properties, such as elastic modulus. In other words, the nominal bond strength misrepresents the actual maximum shear or tensile stresses the specimen resisted at failure. As this sensitivity is more pronounced in the shear test set-up, it was concluded that tensile bond strength tests were still preferable. Moreover, although a shear loading is applied during testing, it was demonstrated that tensile stresses produced by the bending moment are responsible for fracture initiation[22]. Amidst this controversy, shear tests were almost completely substituted by the microtensile test, introduced by Sano et al. [26]. The main character- istic of this test is the reduced specimen size. It is also verified that different values are achieved for different bonding areas: the smaller the area, the higher the bond strength [23]. More recently, a new test method using specimens with reduced dimensions has been advocated by some authors [24,25] as a substitute for the conventional shear test:

the so-called ‘microbond’ or ‘micro-shear’ bond strength test. According to them, this test would allow for testing of small areas, thus permitting a regional mapping or depth profiling of different substrates, and preparing multiple specimens from a same tooth, as in microtensile tests, but without sectioning procedures to obtain sticks or trimming to achieve dumbbell or hour-glass shaped specimens, laboratory procedures that may by themselves induce early micro cracking within the specimen. Studies on stress distribu- tion in conventional shear tests cannot be applied to the micro-shear method. One of the reasons may be the lack of proportionality between the geometrical aspects of both tests, whereas composite and dentin diameters may vary, the adhesive layer thickness will always remain constant. Considering the importance of knowing what a test is actually measuring to ensure proper interpretation of obtained data, finite element analysis be- comes of great usefulness to elucidate the stress states found in bonded interfaces and provide information on the nature of stresses generated within the specimen.

The micro shear bond strength test consist in mounting a specimen with cross section
not exceeding 4mm^{2} on a testing machine as shown in figure. Then, a load is applied
in the radial direction of the restorative material in other produce a stress state in the
specimen which will caused the failure at the adhesive interface of the specimen. As we
already stated, it is necessary to have an adhesive failure (fig2.3) of the specimen in order
to evaluate the tensile bond strength dividing the peak of the shear force registered by

Figure 3.1: Dimensions of a generic specimen for the micro shear bond test

the cross section area of the restorative material. This is done because the restorative material cross section represents the area on which the adhesive is applied and only that area will stick to the dentin. The load is generated by the displacement of the cross head speed of the universal testing machine whose velocity during the test ranges usually from 1mm/min to 5mmm/min.

Figure 3.2: Specimen mounted on the testing machine for the micro shear bond test

### 3.2 Finite Element Model With Tiebreak Contact

Two approaches were used to model and simulate the shear bond strength test in order to characterize the adhesive system. Just like for the case of the microtensile bond strength test, the main difference between the two models built for the shear bond strength test

and corresponding to the two approaches that we used lies in the modelling of the cohesive zone of our models. Here is the description of the first approach based on the modelling of the cohesive zone with the contact known as Tiebreak Contact in LS-DYNA.

### 3.2.1 Geometry And Mesh

The experimental test allowed us to have a clear idea on the geometry of our model.We can see from figure how the experimental test was performed. Therefore, Three solid parts were modelled in LS-PREPOST, then we generated a three dimensional solid mesh from the three parts. In order to have a realistic mesh of our model, the mesh generated

(a) Isometric view (b) side view in the (XY) plane

Figure 3.3: Geometry of the model

from the three parts of our model was different from the point of view of the mesh size.

The table summarizes the mesh size and the dimensions of the main parts of the model.

A coarse mesh was generated from the indentor geometry because we were not interested in any information related to the indentor part such as deformation, stress..etc. A finer mesh instead was generated from the block part representing the dentin and the cylindrical part representing the enamel. This was done in order to have a better contact between the dentine and the enamel. The table 3.1 summarizes the information related to the dimensions on the geometry and the mesh size of each part of the model. In the table, r is the radius of the enamel part while l is the length of the enamel. The indentor was

Parts Dimensions Mesh size

Dentin 7mm × 7mm × 2mm 0.1mm Enamel r = 1mm, l = 2mm 0.05mm

Indentor not important /

Table 3.1: Dimensions of the parts and Mesh size of the elements

modelled in order to reproduce in the best possible way the steel rod which transmits the loading to the specimen. It was necessary to have a knife edge at the indentor tip. The

Figure 3.4: Shear bond test model: The mesh

dimensions related to the indentor were not really important nevertheless, the position of the indentor with respect to the contact area was chosen in order to minimize or even avoid a moment load on the enamel part which would have changed the shear bond strength test to flexural bond strength test.

### 3.2.2 Materials

The experimental model comprises the dentin, the enamel and the indentor which is a steel rod. The dentin and the enamel were considered as linear, homogeneous and isotropic materials and modelled with the material 001-ELASTIC in LS-DYNA. The indentor was considered as a rigid material considering its very high elastic modulus with respect to the two other parts elastic modulus (Tab:3.2). It is worth to precise that by modelling

Parts Young’s Modulus [GPa] Poisson’s Ratio

Dentin 18 0.31

Enamel 69 0.28

Indentor (Steel) 210 0.30

Table 3.2: Properties of the materials

the indentor as a rigid material in LS-DYNA, the indentor will not deform during the simulation and no data related to the indentor will be available during the post processing step. In the other hand, even if the indentor is defined as rigid material, it is necessary to define its mechanical properties such as Young Modulus and Poisson’s ratio for the solver algorithm. This is done in order to compute the contact stiffness between the enamel

and the indentor which is a steel in realty. The adhesive system in this model was not considered as a part just like it is in the realty but, as a specific type of contact between the dentin and the enamel. The table summarizes the material properties of the material used in this model. The choice of the material constitutive laws was motivated by the results that we found in the literature in which previous studies were performed with the aim to define the mechanical properties of these parts.

### 3.2.3 Boundary Conditions

In this numerical model, some nodes of the dentin were constrained as shows the figure.

The constraints enforced on a set of nodes on the dentin aim to prevent the nodal dis- placements along x, y, and z directions. These constraints prevent also the nodal rotations around the x, y and z axis of the reference frame. For what concerns the loading, a motion

Figure 3.5: Boundary Conditions enforced on the model

at a velocity defined on figure 3.6 was prescribed to the indentor in order to simulate the loading condition enforced to the steel rod. It was necessary to constrain all the displace- ments and rotations of the indentor except the translational degree of freedom in the y direction. This was done in order to have the loading force only in the Y direction just like it happens during the experimental test. The velocity of the indentor was chosen in order to accelerate the simulation time and maintained under a certain value at the same time in order to avoid the influence of dynamic effects. Let us recall that the experimen- tal test is performed at a constant velocity of the steel rod equal to 5mm/min while the indentor in the numerical model moves at a velocity which starts from zero and smoothly

Figure 3.6: velocity enforced to the indentor

increases up to reach a maximum value (5mm/s) and remains constant at that value. The simulation is ended before the deceleration of the indentor which is represented by the descendent part of the velocity curve.

### 3.2.4 Contact Between Parts

3.2.4.1 Contact Between the Indentor and the Enamel

The contact between the indentor and the enamel was defined in order to have the trans- mission of the load to the enamel. Without a proper definition of the contact in between some parts having a physical contact in the reality, The solver ignores the interaction be- tween the parts and penetration between the parts does happen. Therefore, In LS-DYNA, a contact is defined by identifying (via parts, part sets, segment sets, and/or node sets) what locations are to be checked for potential penetration of a slave node through a master segment. A search for penetrations, using any of a number of different algorithms, is made every time step. In our case, we defined an AUTOMATIC SURFACE TO SURFACE contact type between the indentor and the enamel. This choice was made because the contact search algorithms employed by automatic contacts make them better-suited than older contact types to handling disjoint meshes.

3.2.4.2 Tiebreak Contact Between the Dentin and the Enamel

The tiebreak contact is one of the most important of this model because it is the one allowing to simulate the adhesive within the model. Therefore, the cohesive zone was modelled using the tiebreak contact. Everything that was said related to the tiebreak contact in the chapter one remains valid for this model. Here are the parameters that we set for the tiebreak:

• NFLS : NFLS represents the normal failure stress of the adhesive. The value of the normal failure stress was unknown but a value of 39 MPa was chosen based on the microtensile bond strength of the adhesive.